# Integration of self-consistent polycrystal plasticity with ... · PDF fileIn this paper, we...

Embed Size (px)

### Transcript of Integration of self-consistent polycrystal plasticity with ... · PDF fileIn this paper, we...

Contents lists available at SciVerse ScienceDirect

Journal of the Mechanics and Physics of Solids

Journal of the Mechanics and Physics of Solids 61 (2013) 20342046

0022-50http://d

n CorrNH 038

E-m

journal homepage: www.elsevier.com/locate/jmps

Integration of self-consistent polycrystal plasticitywith dislocation density based hardening laws withinan implicit finite element framework: Application tolow-symmetry metals

Marko Knezevic a,b,n, Rodney J. McCabe a, Ricardo A. Lebensohn a,Carlos N. Tom a, Cheng Liu a, Manuel L. Lovato a, Bogdan Mihaila a

a Materials Science and Technology Division, Los Alamos National Laboratory, Los Alamos, NM 87545, USAb Department of Mechanical Engineering, University of New Hampshire, Durham, NH 03824, USA

a r t i c l e i n f o

Article history:Received 22 November 2012Received in revised form19 March 2013Accepted 12 May 2013Available online 6 June 2013

Keywords:UraniumConstitutive modelingFinite element methodTextureEBSD

96/$ - see front matter & 2013 Elsevier Ltd.x.doi.org/10.1016/j.jmps.2013.05.005

esponding author at: Department of Mecha24, USA. Tel.: +505 665 7587; fax: +505 667ail address: [email protected] (M. Kn

a b s t r a c t

We present an implementation of the viscoplastic self-consistent (VPSC) polycrystallinemodel in an implicit finite element (FE) framework, which accounts for a dislocation-based hardening law for multiple slip and twinning modes at the micro-scale grain level.The model is applied to simulate the macro-scale mechanical response of a highlyanisotropic low-symmetry (orthorhombic) crystal structure. In this approach, a finiteelement integration point represents a polycrystalline material point and the meso-scalemechanical response is obtained by the mean-field VPSC homogenization scheme. Wedemonstrate the accuracy of the FE-VPSC model by analyzing the mechanical responseand microstructure evolution of -uranium samples under simple compression/tensionand four-point bending tests. Predictions of the FE-VPSC simulations compare favorablywith experimental measurements of geometrical changes and microstructure evolution.Specifically, the model captures accurately the tensioncompression asymmetry of thematerial associated with twinning, as well as the rigidity of the material response alongthe hard-to-deform crystallographic orientations.

& 2013 Elsevier Ltd. All rights reserved.

1. Introduction

Polycrystal plasticity models such as Taylor-type (Kalidindi et al., 1992; Knezevic et al., 2009; Taylor, 1938; Van Houtteet al., 1999) and self-consistent-type models (Lebensohn and Tom, 1993; Lebensohn et al., 2007) have been rigorouslyformulated and extensively used to understand and predict the mechanical response and microstructure evolution in metalssubject to finite strains. The degree of sophistication necessary to accurately model a material generally depends on thecrystal structure and the number and types of deformation modes active in the material. In this paper, we use -uranium(-U) as a model material system to illustrate the predictive capabilities of this modeling framework for low-symmetrymetals. Uranium is an important metal for energy (e.g. metallic nuclear fuels) and defense applications, and is a challengingmaterial to model because of its pronounced mechanical anisotropy. At room temperature, uranium has a low-symmetry

All rights reserved.

nical Engineering, University of New Hampshire, 33 Academic Way, Kingsbury Hall, W119, Durham,8021.ezevic).

www.sciencedirect.com/science/journal/00225096www.elsevier.com/locate/jmpshttp://dx.doi.org/10.1016/j.jmps.2013.05.005http://dx.doi.org/10.1016/j.jmps.2013.05.005http://dx.doi.org/10.1016/j.jmps.2013.05.005http://crossmark.dyndns.org/dialog/?doi=10.1016/j.jmps.2013.05.005&domain=pdfhttp://crossmark.dyndns.org/dialog/?doi=10.1016/j.jmps.2013.05.005&domain=pdfhttp://crossmark.dyndns.org/dialog/?doi=10.1016/j.jmps.2013.05.005&domain=pdfmailto:[email protected]://dx.doi.org/10.1016/j.jmps.2013.05.005

M. Knezevic et al. / J. Mech. Phys. Solids 61 (2013) 20342046 2035

crystal structure (orthorhombic), and polycrystal plasticity requires activation of as many as four different slip modes, and atleast two different deformation twinning modes. To complicate matters, the operating slip and twinning modes exhibit lowmultiplicity and widely different activation stresses. Consequently, the plastic response is highly anisotropic with markedtensioncompression asymmetry and hardening depends strongly on texture and the interactions between the slip andtwin modes. Recently, we showed that a hardening law explicitly based on dislocation density evolution implementedwithin the VPSC homogenization scheme performs well in capturing the anisotropic strain hardening and texture evolutionin -U (Knezevic et al., 2012; McCabe et al., 2010). Subsequently, the VPSC model of -U was extended to account for strain-rate and temperature effects (Knezevic et al., 2013b). Comparison of simulations and experiments in these studies allowedus to infer basic information concerning the various slip and twin mechanisms, their interactions, and their role on strainhardening and texture evolution. It was found that the initial texture plays a significant role in determining the level ofplastic anisotropy, and deformation twinning plays a major role in strain hardening behavior and texture evolution in -U.Hence, it is evident that the accurate modeling of this complex material system requires a crystal-plasticity theoreticalframework that accounts for microstructure evolution, rather than a continuum approach. These early successes provide theincentive for integrating the VPSC-based material subroutine for uranium into a finite element (FE) framework to facilitatepredicting geometrical changes along with microstructure evolution of -U components. Such integration is necessary forengineering structural and process modeling applications.

The strategy of embedding the mean-field VPSC model at the meso-scale level in an implicit FE analysis was recentlydiscussed (Segurado et al., 2012). In an implicit nonlinear FE formulation, the material constitutive model provides the stressand tangent stiffness matrix. In our approach, the tangent stiffness matrix (Jacobian) is obtained analytically and allows forfast convergence towards stress equilibrium. The FE Jacobian is a function of the viscoplastic tangent moduli (which hasalready been calculated as part of the nonlinear self-consistent homogenization scheme), the elastic stiffness of theaggregate, and the FE time increment.

In this paper, we combine these recent advances and present an implementation of the VPSC polycrystalline model inimplicit finite elements that accounts for a dislocation density based hardening law necessary to model the highlyanisotropic response of -U. We demonstrate that the VPSC calculations can be performed in the global FE frame rather thanin the co-rotational frame adopted in the original FE-VPSC implementation (Segurado et al., 2012). The added benefit is thatcrystallographic texture stays in the global frame and thus the field and state variables are not regularly rotated between theglobal and co-rotational frame. Simple compression, simple tension, and simple shear tests on polycrystalline uranium areused to demonstrate the accuracy of the FE-VPSC model in ABAQUS by comparing with the results of the stand-alone VPSCmodel. The -U FE-VPSC model is subsequently used to simulate the mechanical response and texture evolution of -Ucylinders in simple compression and beams in four-point bending deformation experiments. A total of two cylinders andfour beams, classified by the alignment of the sample axis with respect to the rolled plate direction and the loading directionwere experimentally deformed. Quantitative comparisons with experimental measurements of strain fields by digital imagecorrelation (DIC) mapping, geometrical changes captured optically, and texture evolution by electron backscattereddiffraction (EBSD) based orientation imaging are used to demonstrate the predictive capabilities of the model. We findthat the FE-VPSC simulations capture well the strain field, shifts of the neutral axis of the beams, changes in the cross-section geometry and texture evolution during deformation.

2. Modeling framework

In this section, we outline the salient aspects of the micro-scale hardening law based on dislocation densities for -U, theVPSC polycrystal plasticity meso-scale model and its implementation in the macro-scale implicit finite element framework.

2.1. Micro-scale model

Plastic deformation in each grain occurs via the activation of both slip and twin modes. The corresponding slip or twinshear rate, _s on a system, s, is given by the power-law:

_s _o r : m

s

sc

1=m

signr : ms 1

where r is the Cauchy stress deviator, ms is the Schmid tensor associated with slip or twinning system s, _so is the referenceslip rate on system s, m is the rate sensitivity parameter, and sc is the resistance of slip or twinning system s. A rate-sensitivity exponent of 0.1 is taken to be the same for all slip and twinning modes.

Early experiments (Anderson and Bishop, 1962; Daniel et al., 1971; Fisher and McSkimin, 1958; Yoo, 1968) established thefollowing four slip modes (0 1 0)[1 0 0], (0 0 1)[1 0 0], f110g110and f112g021 to operate in -U. In addition to slip,early studies (Cahn, 1951, 1953; Crocker, 1965; Daniel et al., 1971) confirmed the presence of several twin modes, the twomost prevalent in wrought -U being f130g310 and f172g312. Consistent with these experimental findings, we considerall of the above slip and twinning systems as potential systems for accommodating the imposed plastic strain in our model.

The equatio